Effect of Self-etching Adhesives on the Bond Strength of Glass-Ionomer Cements Zahra Jaberi Ansari1, Narges Panahandeh2, Zahra Sadat Tabatabaei Shafiei3, Alireza Akbarzadeh Baghban4 1
Associate professor, Department of Operative Dentistry, Dental School, Shahid Beheshti University of Medical Sciences, Tehran, Iran Assistant Professor, Department of Operative Dentistry, Dental School, Shahid Beheshti University of Medical Science, Tehran, Iran 3 Dentist 4 Associate Professor, Department of Basic Sciences, Faculty of Rehabilitation Sciences, Shahid Beheshti University of Medical Sciences, Tehran, Iran 2
Corresponding author: N. Panahandeh, Department of Operative Dentistry, Dental School, Shahid Beheshti University of Medical Science, Tehran, Iran nargespanah[email protected]
Received: 18 March 2014 Accepted: 14 August 2014
Objective: Statement of Problem: Adequate bond strength between glass ionomer cements and composite resin is necessary for the success of the sandwich technique. Purpose of Study: This study assessed the micro-shear bond strength of composite resin to glass-ionomer cements (GIC) using self-etch adhesives with different pH values. Materials and Methods: One hundred specimens (6×4×2 mm) were made using Fuji II and Fuji II LC GICs and treated with different adhesives as follows: Group 1:Fuji II+ Adper Prompt L-Pop, Group-2: Fuji II+SE bond, Group-3: Fuji II + AdheSE, Group-4:Fuji II+ Protect bond, Group-5: Fuji II + Single bond, Group-6:Fuji II LC+ Adper Prompt LPop, Group-7: Fuji II LC+SE bond, Group-8:Fuji II LC+ AdheSE, Group-9: Fuji II LC+ Protect bond, and Group-10: Fuji II LC+ Single bond. Each group consisted of 10 specimens. A cylinder of Z100 composite resin was placed on each sample and light cured. After 24 hours of water storage (37˚C), the specimens were subjected to micro-shear bond strength tests (0.5 mm/min). Data were analyzed using two-way ANOVA and Tukey’s test. Results: The mean micro-shear bond strength of groups 1-10 was 11.66±1.79, 16.50±1.85, 18.47±1.77, 13.95±1.77, 15.27±1.49, 15.14±0.90, 20.03±1.19, 17.48±3.00, 16.24±1.98 and 16.03±1.49 MPa, respectively. There were significant differences between groups 1 and 7 (P0.05). Fuji II LC showed higher bond strength than Fuji II (P 650 mW/cm2. Groups 2-5 were prepared in an identical procedure. Different bonding agents were used in each group as summarized in Table 2. The only difference was that: To prepare groups 6 to 10 Fuji II LC RMGIC was used instead of Fuji II. Bonding agents were applied according to the protocol used for groups 1 to 5.
Jaberi Ansari et. al
All specimens were mounted on micro-tensile tester (Bisco Inc., USA) using cyanoacrylate glue (Zapite, USA). The crosshead speed of the machine was 0.5 mm/ min. Micro-shear bond strength of specimens was calculated by dividing the load force at specimen fracture (in Newton) by its surface area (mm2) and expressed in MPa. Data were analyzed using two-way ANOVA and Tukey’s test. P-values 0.05). The interaction between the bonding agent and GICs was not significant (F4,90 = 47, P=0.756). DISCUSSION Applying GICs beneath the composite resins (sandwich technique) is a routine restorative technique benefitting from the favorable properties of both materials. Adequate bond strength between the GIC and the composite resin is necessary for the success of this technique . The current study assessed the effect of application of different self-etch bonding agents on the bond strength of composite resin to conventional and resin-modified GICs. The bonding systems used included a strong self-etch bonding agent (Adper Prompt LPop), a moderate self-etch bonding agent (AdheSE), a mild self-etch bonding system (Clearfil SE bond), a fluoridated mild self-etch bonding system (Clearfil Protect bond) and one etch and rinse bonding system (Adper Single bond) as the control, which are all highly popular bonding systems. The obtained data regarding the micro-shear bond strength of different groups showed that Group 1 (Fuji II + Adper Prompt L-Pop) had the least strength values while Group 7 (Fuji II LC + Clearfil SE Bond) showed superior performance in comparison with other groups; the difference between these two groups was stawww.jdt.tums.ac.ir November 2014; Vol. 11, No. 6
tistically significant. No other significant differences were noted. Adper Prompt L-Pop is a strong self-etch bonding system while SE bond is a weak selfetch bonding agent. Kenshima et al. reported that strong self-etch adhesives (low pH) produced the lowest bond strength of resin to dentin . Other investigations have reported that highly acidic self-etching adhesives contain higher solvent contents for promoting complete ionization of the acidic monomers. Thus, the adhesive layer after solvent evaporation will be quite thin, i.e. polymerization may be inadequate due to the formation of an airinhibited layer. Consequently, unpolymerized acidic monomers will increase in this layer. All these factors compromise the polymerizing initiator system interfering with composite polymerization; thus, the bond strength of strong self-etching adhesives will be reduced . Furthermore, the mechanism of action of strong self-etching adhesives is very similar to that of etch and rinse adhesives in which hydroxyapatite minerals are removed from the collagen surface layers following the application of adhesive to the teeth. This results in diminished chemical interactions between minerals, hydroxyapatite and functional monomers in turn ; thus, relying on mere micromechanical bonding in the absence of chemical bonding seems to lead to a lower bond strength, which is another factor that may contribute to the lower bond strength in strong self-etching adhesives. Hinoura et al. reported that low pH bonding agents mostly dissolve the GIC surface and increase micromechanical attachment ; this phenomenon was not observed in the current study. According to Moli et al. Prompt L-Pop contains water as the solvent and solvent evaporation occurs slowly in these systems. Furthermore, the HEMA/water ratio increases when small amounts of solvent (water) are evaporated; the pressure of evaporation is lowered and the remaining water settles at the bond interface. 5 684
Journal of Dentistry, Tehran University of Medical Sciences
All these interfere with complete polymerization . Incomplete polymerization of this bonding system may have also reduced its bond strength to GIC in the current study. Clearfil SE Bond contains 10methacryloxydecyl dihydrogen phosphate (10MDP) as the functional monomer. This system is capable of producing very strong ionized bonds with calcium, which means monomers chemically interact with hydroxyapatite in the dentin and enamel in addition to micromechanical bonding. The rationale may be attributed to the higher bonding strength of the system . This chemical interaction only occurs in mild self-etching adhesives as they cannot produce complete demineralization of the surface, having led to some hydroxyapatite crystals remaining on the collagen. Thus, chemical bonds with carboxylic acid-based monomers or phosphate will develop . As GICs contain calcium, their chemical interaction with acid-etching functional monomers may also improve the bonding strength. Van Meerbeek et al. (2003) stated that mild acidic self-etch bonding adhesives like SE bond are not capable of decalcifying the tooth structure effectively and the remaining hydroxyapatite crystals become involved in additional chemical bonding reactions. The presence of 10-MDP in these bonding systems results in chemical bonding with hydroxyapatite particles. MDP monomer was originally synthesized by Kuraray (Protect bond, SE bond). Its capability of forming strong ionic bonds with mineral ions like calcium may be partly attributed to its intense chemical adhesion to tooth structure . Similarly, application of mild self-etch adhesive to GIC results in minimal flushing of ions. Consequently, remaining cations are available to make strong ionic bonds between the two materials . Li et al. indicated higher shear bond strength of composite to RMGIC than conventional GIC; their findings were in agreement with the results of our study . Different factors may be responsible for the increased shear bond 6685
Jaberi Ansari et. al
strength of RMGICs in comparison with the conventional cements. For example, unpolymerized HEMA on the surfaces of the RMGICs increases the surface wettability of the bonding agent and can increase the bond strength when it polymerizes . Also, unsaturated methacrylate groups on the polyacid chain of polymerized RMGIC may form strong covalent bonds with the resin bonding agent and improve adhesion at the interface of the two materials . Last but not least, the higher cohesive strength of RMGIC might be responsible for the higher bond strength achieved . CONCLUSION Within the limitations of this study, type of self-etch bonding agents had no significant effect on micro-shear bond strength of GICs to composite resin. RMGIC exhibited higher bond strength than the conventional GIC.
REFERENCES 1- Mc Lean JW. Clinical applications of glass-ionomer cements. Oper Dent. 1992;Suppl 5:184-90. 2- Tyas MJ, Toohey A, Clark J. Clinical evaluation of the bond between composite resin and etched glass ionomer cement. Aust Dent J. 1989 Feb;34(1):1-4. 3- Almuammar F, Schulman A, Salama S. Shear bond strength of six restorative materials. J Clin Pediatr Dent 2001Spring; 25(3):221-5. 4- Brackett W, Huget F. The effect of etchant and cement age on the adhesion of resin composite to conventional and resin-modified glass-ionomer cements. Quintessence Int. 1996 Jan;27(1):57-61. 5- Mc Lean JW, Wilson AD. The clinical development of the glass-ionomer cement. Aust Dent J. 1977 Jun;22(3):190-5. 6- Farah S, Orton G, Collard M. Shear bond strength of chemical and light-cured glass ionomer cements bonded to resin composites. Aust Dent J. 1998 Apr;43(2):81-6. www.jdt.tums.ac.ir November 2014; Vol. 11, No. 6
Jaberi Ansari et. al
Effect of Self-etching Adhesives on the Bond Strength of Glass-Ionomer Cements
7- Brown KB1, Swartz ML, Cochran MA,
Phillips RW. The glass ionomer lined cervical composite restoration: an in-vitro investigation. Oper Dent. 1993 Jan-Feb;18(1):17-27. 8- Taggart SE, Pearson GJ. The effect of etching on glass polyalkenoate cements. J Oral Rehabil. 1991 Jan;18(1):31-42. 9- Hinoura K, Suzuki H, Onose H. Factors influencing bond strength between unetched glass ionomers and resins. Oper Dent. 1991 May-Jun;16(3):90-5. 10- Taher NM, Ateyeh NZ. Shear-bond strength of resin modified glass ionomer cement bonded to different tooth-colored restorative materials. J Contemp Dent Pract. 2007 Feb 1;8(2):25-34. 11- Owens BM, Johnson WW. Effect of single step Adhesive on the marginal permeability of class V resin composites. Oper Dent. 2007 Jan-Feb;32(1):67-72. 12- Irie M, Suzuki K, Watts DC. Immediate performance of self-etching versus system adhesive with multiple light-activated restoratives. Dent Mater. 2004 Nov;20(9):873-80. 13- Perdigao J. New developments in dental adhesion. Dent Clin North Am. 2007 Apr;51(2):333-57, viii. 14- Kenshima S, Reis A, Uceda-Gomez N, Tancredo Lde L, Filho LE, Nogueira FN et al. Effect of smear layer thickness and pH of selfetching adhesive system on the bond strength and gap formation to dentin. J Adhes Dent. 2005 Summer;7(2):117-26. 15- Gopikrishna V, Abarajithan M, Krithikadatta J, Kandaswamy D. Shear bond strength evaluation of resin composite bonded to GIC using three different adhesives. Oper Dent. 2009 Jul-Aug;34(4):467-71. doi: 10.2341/08009-L. 16- Arora V, Kundabala M, Parolia A, Thomas MS, Pai V. Comparison of the shear bond strength of RMGIC to a resin composite using different adhesive systems: an in vitro study. J
www.jdt.tums.ac.ir November 2014; Vol. 11, No. 6
Conserv Dent. 2010 Apr;13(2):80-3. doi: 10.4103/0972-0707.66716. 17- Kandaswamy D, Rajan KJ, Venkateshbabu N, Porkodi I. Shear bond strength evaluation of resin composite bonded to glass- ionomer cement using self-etching bonding agents with different Ph: In vitro study. J Conserv Dent. 2012 Jan;15(1):27-31. doi: 10.4103/09720707.92602. 18- McLean JW. New concepts in cosmetic dentistry using glass ionomer cements and composite. CDA J. 1986 Apr;14(4):20-5, 27. 19- Pashley E, Agee KA, Pashley DH, Tay FR. Effects of one versus two applications of an unfilled, all- in- one adhesive on dentin bonding. J Dent. 2002 Feb-Mar;30(2-3):83-90. 20- Moli K, Gartner T, Haller B. Effect of moist bonding on composite/enamel bond strength. Am J Dent. 2002 Apr;15(2):85-90. 21- Van Landuyt KL, Snauwaert J, De Munck J, Peumans M, Yoshida Y, Poitevin A et al. Systematic review of the chemical composition of contemporary dental adhesives. Biomaterials. 2007 Sep;28(26):3757-85. Epub 2007 May 7. 22- De Munck J, Van Landuyt K, Peumans M, Poitevin A, Lambrechts P, Braem M, et al. A critical review of the durability of adhesion to tooth tissue. J Dent Res. 2005 Feb;84(2):11832. 23- Li J, Liu Y, Liu Y, Söremark R, Sundström F. Flexural Strength of resinmodified glass ionomer cements and their bond strength to dental composites. Acta Odontol Scand. 1996 Feb;54(1):55-8. 24- Kerby RE1, Knobloch L. The relative shear bond strength of visible light-curing and chemically curing glass ionomer cement to composite resin. Quintessence Int. 1992 Sep;23(9):641-4. 25- Sidu SK, Watson TF. Resin-Modified glass-ionomer materials. Am J Dent. 1995 Feb;8(1):59-67.